Catalysis Communications 62 (2015) 48–51
Contents lists available at ScienceDirect
Catalysis Communications journal homepage: www.elsevier.com/locate/catcom
Graphene oxide as a facile solid acid catalyst for the production of bioadditives from glycerol esteriﬁcation Xiaoqing Gao a,b, Shanhui Zhu a,⁎, Yongwang Li a,b a b
State Key Laboratory of Coal Conversion, Institute of Coal Chemistry, Chinese Academy of Sciences, Taiyuan 030001, PR China Synfuels China Co. Ltd., Taiyuan 030032, PR China
a r t i c l e
i n f o
Article history: Received 20 September 2014 Received in revised form 26 December 2014 Accepted 6 January 2015 Available online 8 January 2015 Keywords: Glycerol Esteriﬁcation Graphene oxide Bioadditive Diacylglycerol Triacylglycerol
a b s t r a c t Graphene oxide (GO) has proved to be a highly active and reusable solid acid catalyst for glycerol esteriﬁcation with acetic acid in the synthesis of bioadditives diacylglycerol (DAG) and triacylglycerol (TAG). The effects of reaction temperature, molar ratio of acetic acid to glycerol, catalyst amount and reaction time were investigated. A 90.2% combined selectivity of DAG and TAG with complete glycerol conversion was achieved at 120 °C for 6 h over GO. Final characterization shows that the active site of GO is the remaining SO3H group. © 2015 Elsevier B.V. All rights reserved.
1. Introduction The limitation of fossil resources and global concerns regarding environmental issues stimulate the increasing attention for sustainable production of fuels from renewable biomass. Among them, biodiesel has attracted great interest because it possesses nontoxic, biocompatible as well as biodegradable features, and substantially reduces CO2 emission. With the rapid development of biodiesel industry, abundant byproduct glycerol has been produced via the transesteriﬁcation of vegetable oil with low alcohol . Therefore, it is urgent to convert glycerol into valuable chemicals or biofuels to promote the benign development of biodiesel industry. Several innovative strategies have been designed to utilize glycerol involving hydrogenolysis , oxidation , esteriﬁcation [4–6], etheriﬁcation , polymerization  and so on. In this context, one of the most desirable processes is to perform glycerol esteriﬁcation with acetic acid to produce monoacylglycerol (MAG), diacylglycerol (DAG) and triacylglycerol (TAG). These products are widely utilized in cryogenics, biodegradable polyester and cosmetics. Compared with MAG, DAG and TAG own much higher economic value because of their potential applications as valuable liquid fuel additives in improving octane number, cold and viscosity properties . ⁎ Corresponding author at: State Key Laboratory of Coal Conversion, Institute of Coal Chemistry, Chinese Academy of Sciences, Taiyuan 030001, PR China. E-mail address: [email protected]
http://dx.doi.org/10.1016/j.catcom.2015.01.007 1566-7367/© 2015 Elsevier B.V. All rights reserved.
Signiﬁcant acid catalysts have been used for glycerol esteriﬁcation, including sulfated based superacids [9–11], heteropolyacid-based catalysts [12–14], Amberlyst-15 [15–18], tin chloride , zeolite , Y/ SBA-3 , and ZrO2 based solid acids . Regardless of their great advances, most have the drawbacks of rapid deactivation, complex preparation procedures, low reactivity, and expensive costs. To overcome these disadvantages, it is imperative to develop a highly active, inexpensive, robust and sustainable solid acid catalyst for glycerol esteriﬁcation. Recently, graphene and graphene oxide (GO) have gained considerable interest due to their unique physical, chemical and electrical properties . Prepared by Hummer's method, GO undergoes exhaustive oxidation and thus possesses rich oxygen-containing functionalities, such as SO3H, carboxyl, hydroxyl and epoxide groups, which endows it with moderate acidic and oxidizing properties . GO has been employed as an efﬁcient carbocatalyst in hydration , oxidation , Aza-Michael addition  and Friedel–Crafts addition . Recently, GO has demonstrated to be a highly active and reusable solid acid carbocatalyst for furfuryl alcohol alcoholysis in our previous work . Consequently, it is envisaged that GO may be a potential and facile solid acid catalyst for glycerol esteriﬁcation with acetic acid. For the ﬁrst time, GO is reported as an acid catalyst for glycerol esteriﬁcation. Our results indeed show that GO is capable of achieving complete glycerol conversion with ~90% combined selectivity to preferred DAG and TAG. The unprecedented catalytic performance is related to the oxygen-containing groups, particularly the SO3H groups.
X. Gao et al. / Catalysis Communications 62 (2015) 48–51
2. Experimental 2.1. Catalyst preparation GO was prepared by a modiﬁcation to the Hummer's method described elsewhere . Brieﬂy, graphite (5 g) and NaNO3 (2.5 g) were introduced into 115 mL H2SO4 in an ice bath under vigorous stirring. The reaction system was heated to 35 °C and stirred for an additional 30 min after adding 15 g KMnO4. This system was diluted by adding 230 mL deionized water, heated to 98 °C, and followed by adding 700 mL water. The mixture was ﬁltered, washed and dried at 50 °C after introducing 50 mL H2O2 (30 wt.%). The dispersed graphite oxide in water was kept in sonication for 60 min, centrifugated and dried at ambient temperature. The preparation methods of other catalysts (ZSM-48, ZSM-5, H-mordenite, WO3/ZrO2, MoO3/ZrO2, HPW/ZrO2, and Cs2.5PW) were depicted in supporting information. 2.2. Catalyst characterization Scanning Electron Microscopy (SEM) was conducted on a JSM 7001F microscope. EDX spectra were carried out using 20 kV primary electron voltages. The IR spectra were measured by Vertex 70 (Bruker) FT-IR spectrophotometer in the range of 400–4000 cm−1 with a resolution of 4 cm− 1. The samples were mixed with KBr and pressed into translucent disks at room temperature. The S content was measured by elemental microanalysis (EA) (vario MICRO cube, Elemental).
cps/eVV 16 14 12 10 8 S
2.3. Catalytic reaction The catalytic tests for glycerol esteriﬁcation with acetic acid were carried out in a stainless steel autoclave with a magnetic stirring. Typically, 2.0 g glycerol and 13.0 g acetic acid with 0.1 g GO were added into the reactor and then the mixture was heated to the desired temperature for a speciﬁed time. Reaction conditions were changed to investigate the dependence of main variables such as time, reaction temperature, catalyst loading and molar ratio of acetic acid/glycerol. When the reaction was terminated, the reactor was cooled in an icewater bath. After the mixture was separated by centrifugation, the obtained products were diluted with ethanol and analyzed by GC with a FID using a DB-1 capillary column. Corrected area normalization method was used to quantify the products. The assignments of these products were also determined by GC–MS. The conversion of glycerol and selectivity of products were determined by using the following equations. Conversation ð%Þ ¼
Selectivity ð%Þ ¼
4 2 0 1
Fig. 1. Typical SEM–EDS image of GO.
0.378 mmol/g SO3H groups in GO. As displayed in Fig. 2, an intense and broad peak located at ca. 3400 cm−1, corresponding to the stretching mode of OH bond. Additional hydroxyl peaks were located at 1390 cm−1 and 1085 cm−1. The strong bands centered at 1640 cm−1 and 1730 cm−1 (νC_O) were ascribed to carboxylic acid and carbonyl groups. Additionally, the bands at 1260 cm−1 and 800 cm−1 reﬂected the appearance of C–O–C (epoxy) groups .
moles of glycerol ðinÞ−moles of glycerol ðoutÞ moles of all glycerol ðinÞ 100
moles of one product 100 moles of all product
3. Results and discussion 3.1. Catalyst characterization The synthesized GO was characterized by SEM–EDX and FTIR. As indicated by SEM in Fig. 1, GO presented a crumpled and layered structure. EDX spectroscopy showed that GO primarily contained carbon and oxygen, as well as small amounts of sulfur. The large amount of oxygen was an indication of rich oxygen-bearing functionalities. The remaining sulfur conﬁrmed the presence of SO3H group, which can be further corroborated by FTIR (at around 1160 cm−1) . The EA results also showed that the S amount was as high as 1.21 wt.%, corresponding to
Fig. 2. FTIR spectra of fresh and spent GO.
X. Gao et al. / Catalysis Communications 62 (2015) 48–51
Table 1 Catalytic performance of glycerol esteriﬁcation with acetic acid over different catalysts.a Catalyst
Blank GO ZSM-48 ZSM-5 H-mordenite WO3/ZrO2 MoO3/ZrO2 HPW/ZrO2 Cs2.5PW
48.9 98.5 68.0 76.3 75.0 74.2 72.7 73.2 73.0
Selectivity (%) MAG
31.8 15.5 35.7 30.8 35.3 36.9 33.2 38.7 34.9
63.3 60.0 58.0 62.2 58.3 56.7 59.4 55.4 59.2
4.9 24.5 6.3 7.0 6.4 6.4 7.4 5.9 5.9
a Reaction conditions: reaction temperature = 120 °C, molar ratio of glycerol with acetic acid = 1:10, catalyst amount = 0.1 g, reaction time = 1 h.
3.2. Catalytic esteriﬁcation of glycerol Table 1 displays the results from the reaction of glycerol esteriﬁcation with acetic acid over GO and a series of representative solid acid catalysts. Even without the catalyst, 48.9% glycerol was converted to MAG, DAG and TAG, implying that glycerol esteriﬁcation is a selfcatalysis reaction wherein the acidic protons from acetic acid can catalyze this reaction itself. Compared to the blank experiment, ZSM-48 only presented minor promotion for this reaction due to lower acidity. Medium activities were obtained for strong acidic zeolites ZSM-5 and H-mordenite. Other catalysts, such as WO3/ZrO2, MoO3/ZrO2, HPW/ ZrO2 and Cs2.5PW, showed ca. 70% conversion with low TAG selectivity. Surprisingly, excellent reaction performance was achieved for GO, 98.5% conversion and 24.5% TAG selectivity. The combined results clearly demonstrate the high efﬁciency of GO in glycerol esteriﬁcation. GO contains 0.378 mmol/g SO3H groups, which provides an abundance of
Fig. 4. Recycling results of glycerol esteriﬁcation with acetic acid over GO catalysts. Reaction conditions: reaction temperature = 120 °C, molar ratio of glycerol with acetic acid = 1:10, catalyst amount = 0.1 g, reaction time = 6 h.
acidic sites. As glycerol esteriﬁcation is a typical acid-catalyzed reaction, the superior performance of GO should be mainly attributed to the large amounts of strong acidic SO3H groups. Additionally, the unique layered structure facilitates to adsorb reactants and promote the reaction. 3.3. Inﬂuence of reaction conditions Reaction temperature has signiﬁcant impact on the catalytic activity and product distribution. As shown in Fig. 3A, glycerol conversion improved remarkably with the increasing reaction temperature and
Fig. 3. Effect of reaction temperature (A), molar ratio of acetic acid to glycerol (B), catalyst loading (C) and reaction time (D) on the catalytic performance of glycerol esteriﬁcation with acetic acid over GO catalysts. Reaction conditions: reaction temperature = 120 °C, molar ratio of glycerol with acetic acid = 1:10, catalyst amount = 0.1 g, reaction time = 6 h (except the variables).
X. Gao et al. / Catalysis Communications 62 (2015) 48–51
reached 100% at 100 °C over GO catalyst. Simultaneously, the selectivity for TAG increased drastically with the increasing temperature at the expense of MAG and DAG, indicating that the improvement of temperature is instrumental in promoting the further esteriﬁcation of MAG and DAG to produce TAG. Because glycerol consecutive esteriﬁcation is a highly endothermic reaction, higher temperature facilitates to improve the extent of esteriﬁcation . Comparing the effect of temperature, molar ratio of acetic acid to glycerol had minor effect on glycerol conversion (Fig. 3B). GO presented good conversion, 91.0% at low molar ratio of 4:1. Nevertheless, the selectivity to TAG increased obviously with the increase in molar ratio of acetic acid to glycerol. The increase in acetic acid concentration provides more esteriﬁcation agent which undergoes the formation of TAG through further esteriﬁcation from MAG and TAG. As illustrated in Fig. 3C, complete conversion of glycerol was achieved when using only 0.025 g GO, implying that GO is extremely active for glycerol esteriﬁcation. Regarding the selectivity, the enhancement of catalyst loading slightly increased the selectivity to desired TAG. The reaction time dependence of glycerol esteriﬁcation over GO is illustrated in Fig. 3D. Glycerol conversion of 93.8% was obtained within just 30 min and reached 100% after 2 h. As the reaction proceeded, the selectivity to MAG and DAG declined while TAG selectivity increased correspondingly. These reactivity trends implicitly indicate the consecutive feature of glycerol esteriﬁcation. The interaction of acetic acid with proton sites from GO results in the protonation of carbonyl group, which is attacked by glycerol and generated an acylium ion intermediate . This intermediate tends to approach other acetic acid molecule and further proceeds consecutive nucleophilic attack on acetic acid. After reacting for 6 h, the combined selectivity of desired DAG and TAG was up to 90.2% over GO, which is among the best results (Table S1). Compared to the published reports, the combined yield to DAG and TAG is higher than that of PrSO3H–SBA15 , sulfated zirconia , HPW/AC , Y/SBA-3 , and MoOx/TiO2–ZrO2 .
towards glycerol esteriﬁcation to valuable bioadditives. The excellent performance of GO, complete glycerol conversion with 90.2% combined selectivity to DAG and TAG, was mainly attributed to the rich SO3H groups and unique lamellar structure. Moreover, GO presented consistent conversion in consecutive catalytic tests. It can be envisioned that such a cheap and robust solid acid catalyst holds great potential for a wide range of acid-catalyzed reactions.
3.4. Reusability test
As shown in Fig. 4, the recovered GO was reused four times without a decline in catalytic activity. Moreover, the product distribution did not show appreciable change during the complete test. The spent catalyst was characterized by FTIR; the results were compared with the fresh one in Fig. 2. As can be seen, the spent catalyst displayed similar structures with fresh GO, revealing that the oxygen-containing groups were mostly preserved during the reaction. 4. Conclusions Compared to conventional solid acid catalyst, GO prepared by Hummer's method has demonstrated to be a highly active acid catalyst
Acknowledgments The authors gratefully acknowledge the ﬁnancial support of the National Natural Science Foundation of China (no. 21403269).
Appendix A. Supplementary data Supplementary data to this article can be found online at http://dx. doi.org/10.1016/j.catcom.2015.01.007.
References             
           
C.H.C. Zhou, J.N. Beltramini, Y.X. Fan, G.Q.M. Lu, Chem. Soc. Rev. 37 (2008) 527–549. S. Zhu, X. Gao, Y. Zhu, Y. Zhu, H. Zheng, Y. Li, J. Catal. 303 (2013) 70–79. J.A. Sullivan, S. Burnham, Catal. Commun. 56 (2014) 72–75. M.S. Khayoon, B.H. Hameed, Bioresour. Technol. 102 (2011) 9229–9235. S. Zhu, Y. Zhu, X. Gao, T. Mo, Y. Zhu, Y. Li, Bioresour. Technol. 130 (2013) 45–51. S. Zhu, X. Gao, F. Dong, Y. Zhu, H. Zheng, Y. Li, J. Catal. 306 (2013) 155–163. M. Ayoub, M.S. Khayoon, A.Z. Abdullah, Bioresour. Technol. 112 (2012) 308–312. N. Rahmat, A.Z. Abdullah, A.R. Mohamed, Renew. Sustain. Energy Rev. 14 (2010) 987–1000. I. Kim, J. Kim, D. Lee, Appl. Catal. B Environ. 148–149 (2014) 295–303. I. Dosuna-Rodríguez, C. Adriany, E.M. Gaigneaux, Catal. Today 167 (2011) 56–63. P.S. Reddy, P. Sudarsanam, G. Raju, B.M. Reddy, J. Ind. Eng. Chem. 18 (2012) 648–654. A. Patel, S. Singh, Fuel 118 (2014) 358–364. P. Ferreira, I.M. Fonseca, A.M. Ramos, J. Vital, J.E. Castanheiro, Catal. Commun. 12 (2011) 573–576. C.E. Gonçalves, L.O. Laier, A.L. Cardoso, M.J. da Silva, Fuel Process. Technol. 102 (2012) 46–52. L. Zhou, T.-H. Nguyen, A.A. Adesina, Fuel Process. Technol. 104 (2012) 310–318. L. Zhou, E. Al-Zaini, A.A. Adesina, Fuel 103 (2013) 617–625. L.N. Silva, V.L.C. Goncalves, C.J.A. Mota, Catal. Commun. 11 (2010) 1036–1039. V.L.C. Goncalves, B.P. Pinto, J.C. Silva, C.J.A. Mota, Catal. Today 133 (2008) 673–677. C. Gonçalves, L. Laier, M. Silva, Catal. Lett. 141 (2011) 1111–1117. M.S. Khayoon, S. Triwahyono, B.H. Hameed, A.A. Jalil, Chem. Eng. J. 243 (2014) 473–484. P.S. Reddy, P. Sudarsanam, G. Raju, B.M. Reddy, Catal. Commun. 11 (2010) 1224–1228. S. Zhu, C. Chen, Y. Xue, J. Wu, J. Wang, W. Fan, ChemCatChem 6 (2014) 3080–3083. D.R. Dreyer, H.-P. Jia, C.W. Bielawski, Angew. Chem. Int. Ed. 122 (2010) 6965–6968. S. Verma, H.P. Mungse, N. Kumar, S. Choudhary, S.L. Jain, B. Sain, O.P. Khatri, Chem. Commun. 47 (2011) 12673–12675. A. Vijay Kumar, K. Rama Rao, Tetrahedron Lett. 52 (2011) 5188–5191. J. Wang, W. Xu, J. Ren, X. Liu, G. Lu, Y. Wang, Green Chem. 13 (2011) 2678–2681.